Composition Solidus Liquidus (wt% Au) Temperature ( C) Temperature ( C)


 Clifton Booth
 1 years ago
 Views:
Transcription
1 10.4 Given here are the solidus and liquidus temperatures for the copper gold system. Construct the phase diagram for this system and label each region. Composition Solidus Liquidus (wt% Au) Temperature ( C) Temperature ( C) The coppergold phase diagram is constructed below.
2 10.5 Cite the phases that are present and the phase compositions for the following alloys: (a) 25 wt% Pb 75 wt% Mg at 425 C (800 F) (b) 55 wt% Zn 45 wt% Cu at 600 C (1110 F) (c) 7.6 lb m Cu and lb m Zn at 600 C (1110 F) (d) 4.2 mol Cu and 1.1 mol Ag at 900 C (1650 F) (a) For an alloy composed of 25 wt% Pb75 wt% Mg and at 425 C, from Figure 10.20, only the α phase is present; its composition is 25 wt% Pb75 wt% Mg. (b) For an alloy composed of 55 wt% Zn45 wt% Cu and at 600 C, from Figure 10.19, β and γ phases are present, and C β 51 wt% Zn49 wt% Cu C γ 58 wt% Zn42 wt% Cu (c) For an alloy composed of 7.6 lb m Cu and lb m Zn and at 600 C, we must first determine the Cu and Zn concentrations (using Equation 5.6), as C Cu 7.6 lb m 7.6 lb m lb m wt% C Zn lb m 7.6 lb m lb m wt% From Figure 10.19, only the L phase is present; its composition is 95.0 wt% Zn5.0 wt% Cu (d) For an alloy composed of 4.2 mol Cu and 1.1 mol Ag and at 900 C, it is necessary to determine the Cu and Ag concentrations in weight percent. However, we must first compute the masses of Cu and Ag (in grams) using a rearranged form of Equation 5.7: m ' Cu n mcu A Cu (4.2 mol)(63.55 g/mol) g m ' Ag n mag A Ag (1.1 mol)( g/mol) g Now, using Equation 5.6, concentrations of Cu and Ag are determined as follows:
3 C Cu g g g wt% C Ag g wt% g g From Figure 10.7, α and liquid phases are present; and C α 8 wt% Ag92 w% Cu C L 45 wt% Ag55 wt% Cu
4 10.8 Determine the relative amounts (in terms of mass fractions) of the phases for the alloys and temperatures given in Problem therefore W α 1.0. (a) For an alloy composed of 25 wt% Pb75 wt% Mg and at 425 C, only the α phase is present; are (b) For an alloy composed of 55 wt% Zn45 wt% Cu and at 600 C, compositions of the β and γ phases C β 51 wt% Zn49 wt% Cu C γ 58 wt% Zn42 wt% Cu And, since the composition of the alloy, C 0 55 wt% Zn45 wt% Cu, then, using the appropriate lever rule expressions and taking compositions in weight percent zinc W β C γ C C γ C β W γ C 0 C β C γ C β (c) For an alloy composed of 7.6 lb m Cu and lb m Zn (95.0 wt% Zn5.0 wt% Cu) and at 600 C, only the liquid phase is present; therefore, W L 1.0 (d) For an alloy composed of 4.2 mol Cu and 1.1 mol Ag (30.8 wt% Ag69.2 wt% Cu) and at 900 C, compositions of the α and liquid phases are C α 8 wt% Ag92 w% Cu C L 45 wt% Ag55 wt% Cu And, since the composition of the alloy, C wt% Ag69.2 wt% Cu, then, using the appropriate lever rule expressions and taking compositions in weight percent silver W α C L C 0 C L C α
5 W L C 0 C α C L C α
6 10.14 Determine the relative amounts (in terms of volume fractions) of the phases for the alloys and temperatures given in Problems 10.5a and b. Given here are the approximate densities of the various metals at the alloy temperatures: Temperature Density Metal ( C) (g/cm 3 ) Cu Mg Pb Zn This problem asks that we determine the phase volume fractions for the alloys and temperatures in Problems 10.5a and b. This is accomplished by using the technique illustrated in Example Problem 10.3, and also the results of Problems 10.5 and (a) This is a PbMg alloy at 425 C, wherein only the α phase is present. Therefore, V α 1.0. (b) This is a ZnCu alloy at 600 C, wherein C β 51 wt% Zn49 wt% Cu C γ 58 wt% Zn42 wt% Cu W β 0.43 W γ 0.57 ρ Zn 6.67 g/cm 3 ρ Cu 8.68 g/cm 3 Using these data it is first necessary to compute the densities of the β and γ phases using Equation 5.13a. Thus ρ β 100 C Zn (β) + C Cu(β) ρ Zn ρ Cu g/cm g /cm g /cm 3
7 100 ρ γ C Zn (γ) + C Cu(γ) ρ Zn ρ Cu g /cm g /cm g/cm 3 Now we may determine the V β and V γ values using Equation Thus, W β V β W β ρ β ρ β + W γ ρ γ g /cm g /cm g /cm W γ V γ W β ρ β ρ γ + W γ ρ γ g /cm g /cm g /cm
8 10.15 It is desirable to produce a copper nickel alloy that has a minimum noncoldworked tensile strength of 380 MPa (55,000 psi) and a ductility of at least 45%EL. Is such an alloy possible? If so, what must be its composition? If this is not possible, then explain why. From Figure 10.6a, a tensile strength greater than 380 MPa is possible for compositions between about 32 and 90 wt% Ni. On the other hand, according to Figure 10.6b, ductilities greater than 45%EL exist for compositions less than about 13 wt% and greater than about 94 wt% Ni. Therefore, such an alloy is not possible inasmuch, that in order to meet the stipulated criteria: For a TS > 380 MPa For %EL > 45% 32 wt% < C Ni < 90 wt% C Ni < 13 wt% or C Ni > 94 wt%
9 10.16 Briefly explain why, upon solidification, an alloy of eutectic composition forms a microstructure consisting of alternating layers of the two solid phases. Upon solidification, an alloy of eutectic composition forms a microstructure consisting of alternating layers of the two solid phases because during the solidification atomic diffusion must occur, and with this layered configuration the diffusion path length for the atoms is a minimum.
10 10.17 Is it possible to have a magnesium lead alloy in which the mass fractions of primary α and total α are 0.60 and 0.85, respectively, at 460 C (860 F)? Why or why not? In order to make this determination we need to set up the appropriate lever rule expression for each of these quantities. From Figure and at 460 C, C α 41 wt% Pb, C Mg 2 Pb 81 wt% Pb, and C eutectic 67 wt% Pb. For primary α W α' C eutectic C 0 C eutectic C α 67 C Solving for C 0 gives C wt% Pb. Now the analogous expression for total α W α C Mg2 Pb C 0 C Mg2 Pb C α 81 C which yields a value of 47 wt% Pb for C 0. Therefore, since these two C 0 values are different, this alloy is not possible.
11 10.20 For a 64 wt% Zn 36 wt% Cu alloy, make schematic sketches of the microstructure that would be observed for conditions of very slow cooling at the following temperatures: 900 C (1650 F), 820 C (1510 F), 750 C (1380 F), and 600 C (1100 F). Label all phases and indicate their approximate compositions. The illustration below is the CuZn phase diagram (Figure 10.19). A vertical line at a composition of 64 wt% Zn36 wt% Cu has been drawn, and, in addition, horizontal arrows at the four temperatures called for in the problem statement (i.e., 900 C, 820 C, 750 C, and 600 C). On the basis of the locations of the four temperaturecomposition points, schematic sketches of the four respective microstructures along with phase compositions are represented as follows:
12
13 10.29 Consider 3.5 kg of austenite containing 0.95 wt% C, cooled to below 727 C (1341 F). (a) What is the proeutectoid phase? (b) How many kilograms each of total ferrite and cementite form? (c) How many kilograms each of pearlite and the proeutectoid phase form? (d) Schematically sketch and label the resulting microstructure. (a) The proeutectoid phase will be Fe 3 C since 0.95 wt% C is greater than the eutectoid composition (0.76 wt% C). (b) For this portion of the problem, we are asked to determine how much total ferrite and cementite form. Application of the appropriate lever rule expression yields W α C Fe3 C C 0 C Fe3 C C α which, when multiplied by the total mass of the alloy, gives (0.86)(3.5 kg) 3.01 kg of total ferrite. Similarly, for total cementite, W Fe3 C C 0 C α C Fe3 C C α And the mass of total cementite that forms is (0.14)(3.5 kg) 0.49 kg. (c) Now we are asked to calculate how much pearlite and the proeutectoid phase (cementite) form. Applying Equation 10.22, in which C ' wt% C W p 6.70 C 1 ' which corresponds to a mass of (0.97)(3.5 kg) 3.4 kg. Likewise, from Equation W Fe3 C' C 1 ' which is equivalent to (0.03)(3.5 kg) 0.11 kg of the total 3.5 kg mass. (d) Schematically, the microstructure would appear as:
14
15 10.32 Consider 1.5 kg of a 99.7 wt% Fe 0.3 wt% C alloy that is cooled to a temperature just below the eutectoid. (a) How many kilograms of proeutectoid ferrite form? (b) How many kilograms of eutectoid ferrite form? (c) How many kilograms of cementite form? (a) Equation must be used in computing the amount of proeutectoid ferrite that forms. Thus, W α' 0.76 C 0 ' Or, (0.622)(1.5 kg) kg of proeutectoid ferrite forms. (b) In order to determine the amount of eutectoid ferrite, it first becomes necessary to compute the amount of total ferrite using the lever rule applied entirely across the α + Fe 3 C phase field, as W α C Fe3 C C 0 ' C Fe3 C C α which corresponds to (0.958)(1.5 kg) kg. Now, the amount of eutectoid ferrite is just the difference between total and proeutectoid ferrites, or kg kg kg (c) With regard to the amount of cementite that forms, again application of the lever rule across the entirety of the α + Fe 3 C phase field, leads to W Fe3 C C 0 ' C α C Fe3 C C α which amounts to (0.042)(1.5 kg) kg cementite in the alloy.
16 11.2 (a) For the solidification of nickel, calculate the critical radius r* and the activation free energy ΔG* if nucleation is homogeneous. Values for the latent heat of fusion and surface free energy are J/m 3 and J/m 2, respectively. Use the supercooling value found in Table (b) Now calculate the number of atoms found in a nucleus of critical size. Assume a lattice parameter of nm for solid nickel at its melting temperature. (a) This portion of the problem asks that we compute r* and G* for the homogeneous nucleation of the solidification of Ni. First of all, Equation 11.6 is used to compute the critical radius. The melting temperature for nickel, found inside the front cover is 1455 C; also values of H ( 2.53 x 10 9 J/m 3 f ) and γ (0.255 J/m 2 ) are given in the problem statement, and the supercooling value found in Table 11.1 is 319 C (or 319 K). Thus, from Equation 11.6 we have r * 2γT m 1 H f T m T (2)(0.255 J /m2 )( K) J /m K m 1.09 nm For computation of the activation free energy, Equation 11.7 is employed. Thus G * 16 π γ3 T2 m 1 3 H 2 f (T m T) 2 (16)(π)(0.255 J /m2 ) 3 ( K) 2 1 (3)( J /m 3 ) 2 (319 K) J (b) In order to compute the number of atoms in a nucleus of critical size (assuming a spherical nucleus of radius r*), it is first necessary to determine the number of unit cells, which we then multiply by the number of atoms per unit cell. The number of unit cells found in this critical nucleus is just the ratio of critical nucleus and unit cell volumes. Inasmuch as nickel has the FCC crystal structure, its unit cell volume is just a 3 where a is the unit cell length (i.e., the lattice parameter); this value is nm, as cited in the problem statement. Therefore, the number of unit cells found in a radius of critical size is just
17 # unit cells /particle 4 πr *3 3 a 3 4 (π)(1.09 nm) 3 3 (0.360 nm) unit cells Inasmuch as 4 atoms are associated with each FCC unit cell, the total number of atoms per critical nucleus is just
18 11.7 (a) Briefly describe the phenomena of superheating and supercooling. (b) Why do these phenomena occur? (a) Superheating and supercooling correspond, respectively, to heating or cooling above or below a phase transition temperature without the occurrence of the transformation. (b) These phenomena occur because right at the phase transition temperature, the driving force is not sufficient to cause the transformation to occur. The driving force is enhanced during superheating or supercooling.
19 11.10 Using the isothermal transformation diagram for an iron carbon alloy of eutectoid composition (Figure 11.23), specify the nature of the final microstructure (in terms of microconstituents present and approximate percentages of each) of a small specimen that has been subjected to the following time temperature treatments. In each case assume that the specimen begins at 760 C (1400 F) and that it has been held at this temperature long enough to have achieved a complete and homogeneous austenitic structure. (a) Rapidly cool to 400 C (750 F), hold for 500 s, then quench to room temperature. (b) Reheat the specimen in part (a) to 700 C (1290 F) for 20 h. (c) Cool rapidly to 665 C (1230 F), hold for 10 3 s, then quench to room temperature. (d) Rapidly cool to 350 C (660 F), hold for 150 s, then quench to room temperature. This problem asks us to determine the nature of the final microstructure of an ironcarbon alloy of eutectoid composition, that has been subjected to various isothermal heat treatments. Figure is used in these determinations. (a) 100% bainite (b) 100% spheroidite (c) 100% coarse pearlite (d) 50% bainite and 50% martensite
20 11.13 Make a copy of the isothermal transformation diagram for a 1.13 wt% C iron carbon alloy (Figure 11.49), and then on this diagram sketch and label time temperature paths to produce the following microstructures: (a) 6.2% proeutectoid cementite and 93.8% coarse pearlite (b) 50% fine pearlite and 50% bainite (c) 100% martensite (d) 100% tempered martensite Below is shown an isothermal transformation diagram for a 1.13 wt% C ironcarbon alloy, with timetemperature paths that will produce (a) 6.2% proeutectoid cementite and 93.8% coarse pearlite; (b) 50% fine pearlite and 50% bainite; (c) 100% martensite; and (d) 100% tempered martensite.
21 11.16 Name the microstructural products of 4340 alloy steel specimens that are first completely transformed to austenite, then cooled to room temperature at the following rates: (a) C/s, (b) 0.05 C/s, (c) 0.5 C/s, (d) 5 C/s. Figure is used for these determinations. (a) At a cooling rate of C/s, proeutectoid ferrite and pearlite form. (b) At a cooling rate of 0.05 C/s, martensite, ferrite, and bainite form. (c) At a cooling rate of 0.5 C/s, martensite and bainite form. (d) At a cooling rate of 5 C/s, martensite and bainite form.
22 11.D3 An alloy steel (4340) is to be used in an application requiring a minimum tensile strength of 1515 MPa (220,000 psi) and a minimum ductility of 40% RA. Oil quenching followed by tempering is to be used. Briefly describe the tempering heat treatment. We are to consider the tempering of an oilquenched 4340 steel. From Figure 11.35, for a minimum tensile strength of 1515 MPa (220,000 psi) a tempering temperature of less than 400 C (750 F) is required. Also, for a minimum ductility of 40%AR, tempering must be carried out at a temperature greater than about 300 C (570 F). Therefore, tempering must occur at between 300 and 400 C (570 and 750 F) for 1 h.
23
Solution: ΔG = a 3 ΔG v. + 6a 2 γ. Differentiation of this expression with respect to a is as. d ΔG da = d(a3 ΔG v. + d(6a2 γ) = 3a 2 ΔG v.
14:440:407 ch10 Question 10.2: (a) Rewrite the expression for the total free energy change for nucleation (Equation 10.1) for the case of a cubic nucleus of edge length a (instead of a sphere of radius
More information= 62 wt% Ni38 wt% Cu.
92 9.2 (a) From Figure 9.8, the maximum solubility of Pb in Sn at 100 C corresponds to the position of the β (α + β) phase boundary at this temperature, or to about 2 wt% Pb. (b) From this same figure,
More information9.11 Upon heating a leadtin alloy of composition 30 wt% Sn70 wt% Pb from 150 C and utilizing Figure
913 9.8: 9.11 Upon heating a leadtin alloy of composition 30 wt% Sn70 wt% Pb from 150 C and utilizing Figure (a) The first liquid forms at the temperature at which a vertical line at this composition
More informationMATERIALS 101 INTRODUCTION TO STRUCTURE AND PROPERTIES WINTER Problem Set 6 Due: Tuesday, March 6, 11:00 AM
Problem Set 6 Due: Tuesday, March 6, 11:00 AM 1. TTT Diagrams Based on the transformation diagrams for eutectoid steel shown below, what microstructure would result from the following cooling histories?
More informationChapter 10: Phase Transformations
Chapter 10: Phase Transformations ISSUES TO ADDRESS... Transforming one phase into another takes time. Fe C FCC γ (Austenite) Eutectoid transformation Fe 3 C (cementite) + α (ferrite) (BCC) How does the
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationChapter Outline: Phase Transformations in Metals
Chapter Outline: Phase Transformations in Metals Heat Treatment (time and temperature) Microstructure Mechanical Properties Kinetics of phase transformations Multiphase Transformations Phase transformations
More informationIronCarbon Phase Diagram (a review) see Callister Chapter 9
IronCarbon Phase Diagram (a review) see Callister Chapter 9 University of Tennessee, Dept. of Materials Science and Engineering 1 The Iron Iron Carbide (Fe Fe 3 C) Phase Diagram In their simplest form,
More informationIntroduction to Materials Science, Chapter 9, Phase Diagrams. Phase Diagrams. University of Tennessee, Dept. of Materials Science and Engineering 1
Phase Diagrams University of Tennessee, Dept. of Materials Science and Engineering 1 Chapter Outline: Phase Diagrams Microstructure and Phase Transformations in Multicomponent Systems Definitions and basic
More informationProblem Set 7 Materials101 1.) You wish to develop a gold alloy (mostly gold) that can be precipitation strengthened to provide high strength  high conductivity electrical leads to integrated circuits
More informationCHAPTER 9 Part 1. = 5 wt% Sn95 wt% Pb C β. = 98 wt% Sn2 wt% Pb. = 77 wt% Ag23 wt% Cu. = 51 wt% Zn49 wt% Cu C γ. = 58 wt% Zn42 wt% Cu
CHAPTER 9 Part 1 9.5 This problem asks that we cite the phase or phases present for several alloys at specified temperatures. (a) For an alloy composed of 15 wt% Sn85 wt% Pb and at 100 C, from Figure
More informationIntroduction to Iron Metallurgy. Lee Morin Houston Home Metal Shop Club October 2010
Introduction to Iron Metallurgy Lee Morin Houston Home Metal Shop Club October 2010 Book I stole the pictures from We will start with a brief overview! Metals Are Crystals Fundamental geometry of a crystal
More informationIntroduction to Materials Science, Chapter 11, Thermal Processing of Metal Alloys. Chapter 11 Thermal Processing of Metal Alloys
Chapter 11 Thermal Processing of Metal Alloys Designer Alloys: Utilize heat treatments to design optimum microstructures and mechanical properties (strength, ductility, hardness.) Strength in steels correlates
More informationCHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS
41 CHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Vacancies and SelfInterstitials 4.1 In order to compute the fraction of atom sites that are vacant in copper at 1357 K, we must employ Equation
More informationAlloys & Their Phase Diagrams
Alloys & Their Phase Diagrams Objectives of the class Gibbs phase rule Introduction to phase diagram Practice phase diagram Lever rule Important Observation: One question in the midterm Consider the Earth
More informationPhase transformation
Phase transformation Phase Transformation Topics o Basic principles relating to transformations o Kinetics of phase transformation: Nucleation and growth o Metastable and equilibrium state o Shape memory
More information3. Apply phase rule to the two phase field of a binary isomorphous diagram. What conclusion can be drawn?
ecture 1822: Solidification of binary alloys: Solidification of binary alloys: limits of solubility, isomorphous system, lever rule, constitutional super cooling, effect of non equilibrium cooling, eutectic,
More informationIntroduction to Structure and Properties Winter 2005 Final Exam March 17, 2005 TOTAL POINTS 37
Materials 101 Introduction to Structure and Properties Winter 005 Final Exam March 17, 005 Solutions TOTAL POINTS 37 Problem 1: Tensile Test and Plastic Deformation (10 Points) A copper rod is deformed
More informationLecture 19: Eutectoid Transformation in Steels: a typical case of Cellular
Lecture 19: Eutectoid Transformation in Steels: a typical case of Cellular Precipitation Today s topics Understanding of Cellular transformation (or precipitation): when applied to phase transformation
More informationDr. Pulak M. Pandey. paniit.iitd.ac.in/ ~ pmpandey
Dr. Pulak M. Pandey http:// paniit.iitd.ac.in/ ~ pmpandey Metals and alloys may not posses all the desired properties in the finished product. Alloying and heat treatment are two methods which are extensively
More informationCHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS. C Zn A Cu C Zn A Cu C Cu A Zn. (30)(63.55 g /mol) (30)(63.55 g /mol) (70)(65.
HAPTER 4 IMPERFETIONS IN SOLIDS PROBLEM SOLUTIONS wt% u? 4.7 What is the composition, in atom percent, of an alloy that consists of 30 wt% Zn and 70 4.6 as In order to compute composition, in atom percent,
More informationMAE 20 Winter 2011 Assignment 3 solutions
MAE 20 Winter 2011 Assignment 3 solutions 4.3 Calculate the activation energy for vacancy formation in aluminum, given that the equilibrium number of vacancies at 500 C (773 K) is 7.57 10 23 m 3. The
More informationHeat Treatment of Steel
Heat Treatment of Steel Steels can be heat treated to produce a great variety of microstructures and properties. Generally, heat treatment uses phase transformation during heating and cooling to change
More informationThe mechanical properties of metal affected by heat treatment are:
Training Objective After watching this video and reviewing the printed material, the student/trainee will learn the basic concepts of the heat treating processes as they pertain to carbon and alloy steels.
More informationHeat Treatment of Steels : Spheroidize annealing. Heat Treatment of Steels : Normalizing
Heat Treatment of Steels :Recrystallization annealing The carbon and alloy steels were treated at a temperature of about 700 C, which is about 20 C below the eutectoid temperature. The holding time should
More informationBINARY SYSTEMS. Definition of Composition: Atomic (molar) fraction. Atomic percent. Mass fraction. Mass percent (weight percent)
BINARY SYSTEMS Definition of Composition: Atomic (molar) fraction Atomic percent Mass fraction Mass percent (weight percent) na =, x i n = A i i i Weight percent mainly in industry! x at % A = x 100 A
More information14:635:407:02 Homework III Solutions
14:635:407:0 Homework III Solutions 4.1 Calculate the fraction of atom sites that are vacant for lead at its melting temperature of 37 C (600 K). Assume an energy for vacancy formation of 0.55 ev/atom.
More informationv kt = N A ρ Au exp (
42 4.2 Determination of the number of vacancies per cubic meter in gold at 900 C (1173 K) requires the utilization of Equations 4.1 and 4.2 as follows: N v N exp Q v N A ρ Au kt A Au exp Q v kt (6.023
More informationChapter 1 Introduction to Material science & Metallurgy
Chapter 1 Introduction to Material science & Metallurgy 1. Material Science & Metallurgy (21419) State the importance of study of materials science and briefly. Explain Engineering requirements of materials.
More informationModule 34. Heat Treatment of steel IV. Lecture 34. Heat Treatment of steel IV
Module 34 Heat reatment of steel IV Lecture 34 Heat reatment of steel IV 1 Keywords : Austenitization of hypo & hyper eutectoid steel, austenization temperature, effect of heat treatment on structure &
More informationm sugar + m water (wt%) = 77 wt% = m sugar + 1500 g 100 m' sugar m' sugar + 1500 g 100
14:440:407 ch9 Question 9.1 Consider the sugar water phase diagram of Figure 9.1. (a) How much sugar will dissolve in 1500 g water at 90 C (194 F)? (b) If the saturated liquid solution in part (a) is cooled
More informationTHE STRUCTURE OF CRYSTALLINE SOLIDS
CHAPTER 3 THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS Fundamental Concepts 3.1 What is the difference between atomic structure and crystal structure? Atomic structure relates to the number of
More informationSection 3: HEAT TREATMENT
Section 3: HEAT TREATMENT Introduction Objectives of Heat Treatment Heat Treatment is the controlled heating and cooling of metals to alter their physical and mechanical properties without changing the
More informationCHAPTER 11 APPLICATIONS AND PROCESSING OF METAL ALLOYS PROBLEM SOLUTIONS
111 CHAPTER 11 APPLICATIONS AND PROCESSING OF METAL ALLOYS PROBLEM SOLUTIONS Ferrous Alloys 11.1 This question asks that we list four classifications of steels, and, for each, to describe properties and
More informationPhase. Gibbs Phase rule
Phase diagrams Phase A phase can be defined as a physically distinct and chemically homogeneous portion of a system that has a particular chemical composition and structure. Water in liquid or vapor state
More information14:635:407:02 Homework III Solutions
14:635:407:02 Homework III Solutions 4.1 Calculate the fraction of atom sites that are vacant for lead at its melting temperature of 327 C (600 K). Assume an energy for vacancy formation of 0.55 ev/atom.
More informationModule 4 Design for Assembly IIT BOMBAY
Module 4 Design for Assembly Lecture Design for Heat Treatment 7 Instructional objectives By the end of this lecture, the student will learn 1. different heat treatment processes, 2. application of various
More informationLABORATORY EXPERIMENTS TESTING OF MATERIALS
LABORATORY EXPERIMENTS TESTING OF MATERIALS 1. TENSION TEST: INTRODUCTION & THEORY The tension test is the most commonly used method to evaluate the mechanical properties of metals. Its main objective
More information(10 4 mm 2 )(1000 mm 3 ) = 10 7 mm = 10 4 m = 6.2 mi
14:440:407 Fall 010 Additional problems and SOLUTION OF HOMEWORK 07 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 To provide
More information5 Some standard heat treatments
Part VI. : Heat treatment Module 5 : Some standard heat treatments 5 Some standard heat treatments 5.1 Annealing Consider the TTT diagram as shown in Fig. 9 and the cooling curves imposed on the TTT diagram.
More informationHW 8. G = a 3 G v. 6a 2. Problem a. To Find:
HW 8 Problem 10. a. To Find: (a) The expression for total free energy change for a cubic nucleus, critical cube edge length, a*, and G* (b) Compare G* for a cube with that for a sphere b. Given: Nucleus
More informationMaterials Science and Engineering Department MSE , Sample Test #1, Spring 2010
Materials Science and Engineering Department MSE 200001, Sample Test #1, Spring 2010 ID number First letter of your last name: Name: No notes, books, or information stored in calculator memories may be
More informationChapter 8. Phase Diagrams
Phase Diagrams A phase in a material is a region that differ in its microstructure and or composition from another region Al Al 2 CuMg H 2 O(solid, ice) in H 2 O (liquid) 2 phases homogeneous in crystal
More informationCHAPTER 3 THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS
CHAPTER THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS Fundamental Concepts.6 Show that the atomic packing factor for HCP is 0.74. The APF is just the total sphere volumeunit cell volume ratio.
More informationPhase Equilibria & Phase Diagrams
Phase Equilibria & Phase Diagrams Week7 Material Sciences and Engineering MatE271 1 Motivation Phase diagram (Ch 9) Temperature Time Kinematics (Ch 10) New structure, concentration (mixing level) (at what
More informationUNIVERSITY OF CALIFORNIA College of Engineering Department of Materials Science & Engineering MSE 121. Spring Semester 2008 Professor R.
UNIVERSITY OF CALIFORNIA College of Engineering Department of Materials Science & Engineering MSE 121 Spring Semester 2008 Professor R. Gronsky Exam Instructions Please PRINT your name in the box above
More informationCHAPTER 19 THERMAL PROPERTIES PROBLEM SOLUTIONS
191 CHAPTER 19 THERMAL PROPERTIES PROBLEM SOLUTIONS Heat Capacity 19.1 The energy, E, required to raise the temperature of a given mass of material, m, is the product of the specific heat, the mass of
More informationExperiment: Heat Treatment  Quenching & Tempering
Experiment: Heat Treatment  Quenching & Tempering Objectives 1) To investigate the conventional heat treatment procedures, such as quenching and annealing, used to alter the properties of steels. SAE
More informationTeach Yourself Unit 2: Phase diagrams and phase transformations
Teach Yourself Unit 2: Phase diagrams and phase transformations Contents Introduction and synopsis A.2 PART 1: Key terminology A.3 PART 2: Simple phase diagrams, and how to read them A.7 PART 3: The ironcarbon
More informationPhase Transformations in Metals and Alloys
Phase Transformations in Metals and Alloys THIRD EDITION DAVID A. PORTER, KENNETH E. EASTERLING, and MOHAMED Y. SHERIF ( г йс) CRC Press ^ ^ ) Taylor & Francis Group Boca Raton London New York CRC Press
More informationFull Density Properties of Low Alloy Steels
Full Density Properties of Low Alloy Steels Michael L. Marucci & Arthur J. Rawlings Hoeganaes Corporation, Cinnaminson, NJ Presented at PM 2 TEC2005 International Conference on Powder Metallurgy and Particulate
More informationBinary phase diagrams
inary phase diagrams inary phase diagrams and ibbs free energy curves inary solutions with unlimited solubility Relative proportion of phases (tie lines and the lever principle) Development of microstructure
More informationPhysics 610/Chemistry 678 Semiconductor Processing and Characterization Quiz I July 18, 2014
Physics 610/Chemistry 678 Semiconductor Processing and Characterization Quiz I July 18, 2014 Part I: Shortanswer questions on basic principles. (5 points each) 1. Briefly describe the CZ method and the
More informationComparison of Three NiHard I Alloys
Comparison of Three NiHard I Alloys Ö. N. Do an 1, J.A. Hawk 1, and J.Rice 2 1 U.S. Department of Energy, Albany Research Center, Albany, Oregon 2 Texaloy Foundry Co., Inc., Floresville, Texas Keywords:
More informationSolidliquid Interface Energy of Metals at Melting Point and Undercooled State
Materials ransactions, Vol. 43, No. 4 (2002) pp. 721 to 726 c 2002 he Japan Institute of Metals Solidliquid Interface Energy of Metals at Melting Point and Undercooled State Zengyun Jian 1, Kazuhiko Kuribayashi
More information1. Introduction to thermodynamics a. What is thermodynamics?
1. Introduction to thermodynamics a. What is thermodynamics? Thermodynamics is a description of material properties as a function of state. What do we mean by state? A macroscopic state of a homogeneous
More informationMassachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139
Massachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139 2.002 Mechanics and Materials II Spring 2004 Laboratory Module No. 5 Heat Treatment of Plain Carbon and Low
More informationCHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS
71 CHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 The dislocation density is just the total dislocation length
More informationDevelopment of HighStrength Steel Wire with Superior Weldability
INDUSTRIAL MATERIALS Development of HighStrength Steel Wire with Superior Weldability Hiromu IzumIda*, Kenichi SHImIzu, Shinei TaKamura, Yasuhiro SHImoda, osamu momozawa and Teruyuki murai Highcarbon
More informationSteam Turbine Castings
Steam Turbine Castings Components for coal fired steam turbine applications have to endure arduous high stress and temperature environments. These castings within the pressure barrier of the turbine have
More informationAPI X80 Grade Electric Resistance Welded Pipe with Excellent Low Temperature Toughness
API X80 Grade Electric Resistance Welded Pipe with Excellent Low Temperature Toughness JFE TECHNICAL REPORT No. 18 (Mar. 2013) NAKATA Hiroshi *1 KAMI Chikara *2 MATSUO Nobuyuki *3 Abstract: This paper
More informationMATERIALS SCIENCE AND ENGINEERING
Complete Solutions to Selected Problems to accompany MATERIALS SCIENCE AND ENGINEERING AN INTRODUCTION Sixth Edition William D. Callister, Jr. The University of Utah John Wiley & Sons, Inc. Copyright 2003
More informationCHROMIUM STEEL POWDERS FOR COMPONENTS. JEANETTE LEWENHAGEN Höganäs AB, Sweden
CHROMIUM STEEL POWDERS FOR COMPONENTS JEANETTE LEWENHAGEN Höganäs AB, Sweden KEYWORDS Prealloyed steel powder, chromium, PM ABSTRACT Chromium as an alloying element is of great interest due to its low
More informationThe ClausiusClapeyron Equation:
Chapter 10 Solid Solutions and Phase Equilibrium What is a phase? Phase Diagram Basics A phase diagram represents what phases are present at a given pressure, temperature and composition. Virtual maps
More informationLead/Tin Solder Lab. 1. Select a labeled cup(s) and sign your names on the table of lead/tin percentages.
Lead/Tin Solder Lab 1. Select a labeled cup(s) and sign your names on the table of lead/tin percentages. 2. Mass out 50 grams total of your assigned lead and tin alloy. 3. Melt the metals together in an
More informationCrystal Structure of Aluminum, Zinc, and their Alloys By: Omar Fajardo Sebastian Henao Devin Baines ENGR45, F2014, SRJC
Crystal Structure of Aluminum, Zinc, and their Alloys By: Omar Fajardo Sebastian Henao Devin Baines ENGR45, F2014, SRJC Purpose The purpose of this experiment was to examine and observe the microstructure
More informationHIGH STRENGTH DUCTILE IRON PRODUCED BY THE ENGINEERED COOLING: PROCESS CONCEPT
IJMC142442 HIGH STRENGTH DUCTILE IRON PRODUCED BY THE ENGINEERED COOLING: PROCESS CONCEPT Copyright 215 American Foundry Society Abstract Simon N. Lekakh Missouri University of Science and Technology,
More informationIn order to solve this problem it is first necessary to use Equation 5.5: x 2 Dt. = 1 erf. = 1.30, and x = 2 mm = 2 103 m. Thus,
5.3 (a) Compare interstitial and vacancy atomic mechanisms for diffusion. (b) Cite two reasons why interstitial diffusion is normally more rapid than vacancy diffusion. Solution (a) With vacancy diffusion,
More information5.6: Characteristic Physical Properties pg. 192
5.6: Characteristic Physical Properties pg. 192 Key Concepts: 1. Physical properties are characteristics that can be determined without changing the composition of the substance. 3. Pure substances have
More informationImperfections in atomic arrangements
MME131: Lecture 8 Imperfections in atomic arrangements Part 1: 0D Defects A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Occurrence and importance of crystal defects Classification
More informationINFLUENCE OF THERMOMECHANICAL TREATMENT ON THE STEEL C45 FATIGUE PROPERTIES
COMATTECH 2005 TRNAVA, 2021 October 2005 INFLUENCE OF THERMOMECHANICAL TREATMENT ON THE STEEL C45 FATIGUE PROPERTIES Jiří MALINA 1+2, Hana STANKOVÁ 1+2, Jaroslav DRNEK 3, Zbyšek NOVÝ 3, Bohuslav MAŠEK
More informationSolution for Homework #1
Solution for Homework #1 Chapter 2: Multiple Choice Questions (2.5, 2.6, 2.8, 2.11) 2.5 Which of the following bond types are classified as primary bonds (more than one)? (a) covalent bonding, (b) hydrogen
More informationStrength and Stiffness
Strength and Stiffness Stress = load/area is applied to a material by loading it Strain = deformation/length a change of shape (dimensions and twist angles) is its response Stiffness = stress/strain is
More informationCONCEPT CHECK QUESTIONS AND ANSWERS. Chapter 2 Atomic Structure and Interatomic Bonding
CONCEPT CHECK QUESTIONS AND ANSWERS Chapter 2 Atomic Structure and Interatomic Bonding Concept Check 2.1 Question: Why are the atomic weights of the elements generally not integers? Cite two reasons. Answer:
More informationPOSSIBILITY OF INDIRECT HARDNESS TESTING OF DUPLEX STAINLESS STEEL
1 POSSIBILITY OF INDIRECT HARDNESS TESTING OF DUPLEX STAINLESS STEEL István Mészáros Associate professor, Department of Materials Science and Engineering H1111 Budapest, Goldmann tér 3. Summary In this
More informationWelcome to the World of Chemistry
Welcome to the World of Chemistry The Language of Chemistry CHEMICAL ELEMENTS  pure substances that cannot be decomposed by ordinary means to other substances. Aluminum Bromine Sodium The Language of
More informationExam # 1 CH 100, Introductory Chemistry, Fall, 2003 Name
Exam # 1 CH 100, Introductory Chemistry, Fall, 2003 Name Be sure to show your set up for all mathematical problems. Your answers must have the correct number of significant digits and the correct units.
More informationEFFECT OF COPPER ALLOY ADDITION METHOD ON THE DIMENSIONAL RESPONSE OF SINTERED FECUC STEELS
EFFECT OF COPPER ALLOY ADDITION METHOD ON THE DIMENSIONAL RESPONSE OF SINTERED FECUC STEELS Michael L. Marucci and Francis G. Hanejko Hoeganaes Corporation Cinnaminson, NJ 08077  USA Abstract FeCuC
More informationEstimating the Eutectic Composition of Simple Binary Alloy System Using Linear Geometry
Estimating the Eutectic Composition of Simple Binary Alloy System Using Linear Geometry Muhammed Olawale Hakeem AMUDA * and Raymond Otito AKABEKWA Department of Metallurgical and Materials Engineering
More informationHeat Treating of Nonferrous Alloys
Metallogr. Microstruct. Anal. (2013) 2:190 195 DOI 10.1007/s1363201300748 TUTORIAL Heat Treating of Nonferrous Alloys Howard E. Boyer Ó American Society for Metals 1984 The reader should understand
More informationMSE 528  PRECIPITATION HARDENING IN 7075 ALUMINUM ALLOY
MSE 528  PRECIPITATION HARDENING IN 7075 ALUMINUM ALLOY Objective To study the time and temperature variations in the hardness and electrical conductivity of AlZnMgCu high strength alloy on isothermal
More informationProduction of ductile iron castings without feeders
Production of ductile iron castings without feeders Possibilities of producing ductile iron castings in green sand mould without feeders by means of "ingate" feeding and control of the graphite precipitation
More informationHydrocarbon Molecules Polymer Molecules The Chemistry of Polymer Molecules
141 CHAPTER 14 POLYMER STRUCTURES PROBLEM SOLUTIONS Hydrocarbon Molecules Polymer Molecules The Chemistry of Polymer Molecules 14.1 The repeat unit structures called for are sketched below. (a Polychlorotrifluoroethylene
More informationCHAPTER 3 THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS
HPTER THE STRUTURE OF RYSTLLINE SOLIDS PROBLEM SOLUTIONS Fundamental oncepts.1 What is the difference between atomic structure and crystal structure? tomic structure relates to the number of protons and
More informationUNIT (2) ATOMS AND ELEMENTS
UNIT (2) ATOMS AND ELEMENTS 2.1 Elements An element is a fundamental substance that cannot be broken down by chemical means into simpler substances. Each element is represented by an abbreviation called
More informationHEAT TREATMENT OF STEEL
HEAT TREATMENT OF STEEL Heat Treatment of Steel Most heat treating operations begin with heating the alloy into the austenitic phase field to dissolve the carbide in the iron. Steel heat treating practice
More informationClassification of Steels CMn Steels: HighStrength LowAlloy Steels:
Classification of Steels CMn Steels: Lowcarbon steels contain up to 0.30% C. Mediumcarbon steels (up to 0.6%) Highcarbon steels (contain from 0.60 to 1.00% C ) Ultrahighcarbon steels (1.25 to 2%)
More informationObjectives/Introduction Extraction of zinc Physical properties of zinc Zinc casting alloys Wrought zinc alloys Engineering design with zinc alloys
Lecture 7 Zinc and its alloys Subjects of interest Objectives/Introduction Extraction of zinc Physical properties of zinc Zinc casting alloys Wrought zinc alloys Engineering design with zinc alloys Objectives
More informationDr. Alaa A. The Iraqi Journal For Mechanical And Material Engineering, Vol. 10,No. 1, 2010
Dr. Alaa A. The Iraqi Journal For Mechanical And Material Engineering, Vol. 10,No. 1, 2010 1.1 Metallurgy of gray cast iron: Most of industrial automobiles companies produced the brake rotor part from
More information8. Technical Heat Treatment
8. Technical Heat Treatment 8. Technical Heat Treatment 95 6 cm 4 2 02 4 C 400 C C 614 1210 86 42 0 2 cm 6 723 C temperature C 1750 750 250 When welding a workpiece, not only the weld itself,
More informationPostWeld Heat Treatment Case Studies
PostWeld Heat Treatment Case Studies Khaleel Ahmed and J. Krishnan Centre for Design and Manufacture Bhabha Atomic Research Centre Introduction H EAT TREATMENT IS AN IMPORTANT operation in the final fabrication
More informationWELDING AND COATING METALLURGY
WELDING AND COATING METALLURGY 1 INTRODUCTION 4 1.1 ROLE OF CARBON IN STEEL 4 1.2 WELDABILITY OF STEELS 5 2 CRYSTAL STRUCTURE 7 2.1 SOLUBILITY OF CARBON 8 3 IRON  IRON CARBIDE PHASE DIAGRAM 9 3.1 AUSTENITE
More informationManufacturing Processes. Casting. Associate Professor SuJin Kim. School of Mechanical Engineering Gyeongsang National University.
Associate Professor SuJin Kim School of Mechanical Engineering Gyeongsang National University Outline 1. Physics 2. Sand 3. Investment 4. Die 5. Cost/Quality is a manufacturing process by which a liquid
More informationEffect of Heat Treatment on the Microstructure and Mechanical Properties of Steel
金属材料及热处理 学生实验报告范例课程编号 :030107 课程主讲及实验课指导教师 : 刘国权黄鹏 Effect of Heat Treatment on the Microstructure and Mechanical Properties of Steel Song Zhen 40531165 University of Science and Technology Beijing, Dept.of
More informationDevelopment of a High Performance NickelFree P/M Steel. Bruce Lindsley. Senior Materials Engineer, Hoeganaes Corporation, Cinnaminson, NJ 08077, USA
Development of a High Performance NickelFree P/M Steel Bruce Lindsley Senior Materials Engineer, Hoeganaes Corporation, Cinnaminson, NJ 08077, USA Abstract A developmental nickelfree P/M steel containing
More informationSome Data. Iron & Steel 61 Non ferrous 9.5 Plastics 11.5 Glass 3.0 Rubber 5.0 Other 10.0 Total weight / kg 901
Some Data Mg Al Ti Fe Density / g cm 3 1.74 2.7 4.51 7.87 Modulus / GPa 45 70 120 210 Specific Modulus / GPa cm 3 g 1 25.9 26 26 27 Melting Temperature / C 650 660 1670 1535 Crystal Structure (300 K) h.c.p.
More informationFor a two dimensional electron gas confined within a square region of sides a we have:
EE145 Spring 00 Homework 4 Prof. Ali Shakouri Chapter 4 *4.6 Density of states for a twodimensional electron gas Second Edition ( 001 McGrawHill) Consider a twodimensional electron gas in which the
More informationDevelopment of API X80 Grade Electric Resistance Welding Line Pipe with Excellent Low Temperature Toughness
JFE TECHNICAL REPORT No. 12 (Oct. 2008) Development of API X80 Grade Electric Resistance Welding Line Pipe with Excellent Low Temperature Toughness NAKATA Hiroshi *1 KAMI Chikara *2 MATHUO Nobuyuki *3
More informationSteel and cast iron. Chapter Chapter 112
Steel and cast iron Chapter 111 Chapter 112 1 Taxonomy of Metals Metal Alloys Ferrous Steels Cast Irons
More informationTHE STRUCTURE OF CRYSTALLINE SOLIDS. IE114 Materials Science and General Chemistry Lecture3
THE STRUCTURE OF CRYSTALLINE SOLIDS IE114 Materials Science and General Chemistry Lecture3 Outline Crystalline and Noncrystalline Materials 1) Single, Polycrystalline, Noncrystalline solids 2) Polycrystalline
More information